#=======================================================================
data_global
#=======================================================================

_audit_creation_method                   'Jana2006 Version : 17/09/2018'

# SUBMISSION DETAILS

_publ_contact_author_name                'Dr Dennis Wiedemann'
_publ_contact_author_id_orcid            0000-0001-6294-3205
_publ_contact_author_address
;
Institut für Chemie
Technische Universität Berlin
Straße des 17. Juni 135
10623 Berlin
Germany
;
_publ_contact_author_email               dennis.wiedemann@chem.tu-berlin.de
_publ_contact_author_fax                 '+49 30 314-79656'
_publ_contact_author_phone               '+49 30 314-26178'

_publ_requested_journal
'Acta Crystallogr.,Sect.B:Struct.Sci.,Cryst.Eng. and Mat.'

#=======================================================================

# TITLE AND AUTHOR LIST

_publ_section_title
;
The Inverse Perovskite BaLiF₃: Single-Crystal Neutron Diffraction and
 Analyses of Potential Ion Pathways
;
_publ_section_title_footnote             .

loop_
 _publ_author_name
 _publ_author_footnote
 _publ_author_address
'Wiedemann, Dennis' .
;
Institut für Chemie
Technische Universität Berlin
Straße des 17. Juni 135
10623 Berlin
Germany
;
'Meutzner, Falk'
;
also at:
Samara National Research University
Moskovskoye Shosse 34
443086 Samara
Russian Federation
;
;
Institut für Experimentelle Physik
TU Bergakademie Freiberg
Leipziger Straße 23
09596 Freiberg
Germany
;
'Fabelo, Oscar' .
;
Institut Laue-Langevin
71 Avenue des Martyrs, CS 20156
38042 Grenoble Cedex 9
France
;
'Ganschow, Steffen' .
;
Leibniz-Institut für Kristallzüchtung
Max-Born-Straße 2
12489 Berlin
Germany
;

#=======================================================================

_publ_section_references
;
Filhol, A. (1988). RAFD9 -- Program for the Refinement of the UB Matrix,
 Wavelength, Cell Parameters and Instrument Zero-Shifts in a Single-Crystal
 Diffraction Experiment. Institut Laue-Langevin, Grenoble, France.

Institut Laue-Langevin (2016). NOMAD. Institut Laue-Langevin, Grenoble, France.

Lehmann, M.S. & Larsen, F.K. (1974). Acta Cryst. A30, 580-584. 

Momma, K. & Izumi, F. (2011). J. Appl. Cryst. 44, 1272-1276.

Palatinus, L. & Chapuis, G. (2007). J. Appl. Cryst. 40, 786-790.

Petříček, V., Dušek, M. & Palatinus, L. (2014). Z. Kristallogr.
 -- Cryst. Mater. 229, 345-352.

Sheldrick, G. (2015). Acta Cryst. C71, 3-8.

Wilkinson, C., Khamis, H.W., Stansfield, R.F.D. & McIntyre, G.J. (1988).
 J. Appl. Cryst. 21, 471-478.
;

#=======================================================================
data_BaLiF3-rt
#=======================================================================

_database_code_CSD                       434514

# CHEMICAL DATA

_chemical_name_systematic                'barium lithium fluoride oxide'
_chemical_name_structure_type            Perovskite-CaTiO₃
_chemical_formula_iupac                  'Ba Li F2.80 O0.10'
_chemical_formula_sum                    'Ba F2.80 Li O0.10'
_chemical_formula_weight                 199.1
_chemical_compound_source                synthetic

#=======================================================================

# CRYSTAL DATA

_symmetry_cell_setting                   cubic
_symmetry_space_group_name_H-M           'P m -3 m'
_symmetry_space_group_name_Hall          '-P 4 2 3'
_symmetry_Int_Tables_number              221

loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -x,-y,z
 3   -x,y,-z
 4   x,-y,-z
 5   z,x,y
 6   z,-x,-y
 7   -z,-x,y
 8   -z,x,-y
 9   y,z,x
 10  -y,z,-x
 11  y,-z,-x
 12  -y,-z,x
 13  y,x,-z
 14  -y,-x,-z
 15  y,-x,z
 16  -y,x,z
 17  x,z,-y
 18  -x,z,y
 19  -x,-z,-y
 20  x,-z,y
 21  z,y,-x
 22  z,-y,x
 23  -z,y,x
 24  -z,-y,-x
 25  -x,-y,-z
 26  x,y,-z
 27  x,-y,z
 28  -x,y,z
 29  -z,-x,-y
 30  -z,x,y
 31  z,x,-y
 32  z,-x,y
 33  -y,-z,-x
 34  y,-z,x
 35  -y,z,x
 36  y,z,-x
 37  -y,-x,z
 38  y,x,z
 39  -y,x,-z
 40  y,-x,-z
 41  -x,-z,y
 42  x,-z,-y
 43  x,z,y
 44  -x,z,-y
 45  -z,-y,x
 46  -z,y,-x
 47  z,-y,-x
 48  z,y,x

_cell_length_a                           3.9978(2)
_cell_length_b                           3.9978(2)
_cell_length_c                           3.9978(2)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        90
_cell_volume                             63.894(10)
_cell_formula_units_Z                    1

_cell_measurement_reflns_used            126
_cell_measurement_theta_min              6.05
_cell_measurement_theta_max              48.53
_cell_measurement_temperature            300.00(3)

_exptl_crystal_density_diffrn            5.1737
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            'not measured'
_exptl_crystal_F_000                     19.582

_exptl_absorpt_coefficient_mu            0.052
_exptl_crystal_description               cube
_exptl_crystal_size_max                  5.00
_exptl_crystal_size_mid                  5.00
_exptl_crystal_size_min                  5.00
_exptl_crystal_colour                    colourless
_exptl_absorpt_correction_type           gaussian
_exptl_absorpt_process_details
'Jana2006 (Petříček et al., 2014)'
_exptl_absorpt_correction_T_min          0.9747
_exptl_absorpt_correction_T_max          0.9777

loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 1  0  0  0.25
-1  0  0  0.25
 0  1  0  0.25
 0 -1  0  0.25
 0  0  1  0.25
 0  0 -1  0.25

#=======================================================================

# EXPERIMENTAL DATA

_diffrn_ambient_temperature              300.00(3)
_diffrn_ambient_environment              vacuum
_diffrn_source                           'nuclear reactor'
_diffrn_source_type                      'ILL high-flux reactor, beam H3'
_diffrn_source_size                      '0.6 \\times 0.6 cm^2^'
_diffrn_source_take-off_angle            56.30
_diffrn_radiation_probe                  neutron
_diffrn_radiation_type                   neutron
_diffrn_radiation_wavelength             0.83860
_diffrn_radiation_monochromator          'Cu 220'
_diffrn_radiation_filter_edge            0.425
_diffrn_measurement_device               'four-circle diffractometer'
_diffrn_measurement_device_type
'D9 position-sensitive detector diffractometer'
_diffrn_measurement_device_details
;
 Eulerian cradle with offset χ circle
;
_diffrn_detector                         '^3^He counter'
_diffrn_detector_type                    'ILL bidim 64mm'
_diffrn_detector_details
;
area detector with pixel size: 2 × 2 mm², 0.25° × 0.25°; pixel
 count: 32 × 32, sensitive area: 64 × 64 mm²
;
_diffrn_detector_area_resol_mean         0.5
_diffrn_measurement_method               'ω and ω-2θ scans'
_diffrn_measurement_specimen_support
;
titanium pin with high-temperature alumina-filled ceramic adhesive
 (Ceramabond 552)
;

_diffrn_reflns_number                    364
_diffrn_reflns_theta_min                 6.02
_diffrn_reflns_theta_max                 57.74
_diffrn_reflns_theta_full                57.74
_diffrn_measured_fraction_theta_max      1.00
_diffrn_measured_fraction_theta_full     1.00
_diffrn_reflns_av_R_equivalents          0.0191
_diffrn_reflns_av_unetI/netI             0.0044
_diffrn_reflns_limit_h_min               -4
_diffrn_reflns_limit_h_max               8
_diffrn_reflns_limit_k_min               -4
_diffrn_reflns_limit_k_max               8
_diffrn_reflns_limit_l_min               0
_diffrn_reflns_limit_l_max               8
_diffrn_reflns_reduction_process         ?

_diffrn_standards_number                 1
_diffrn_standards_interval_count         80
_diffrn_standards_decay_%                -2.8(18)

loop_
 _diffrn_standard_refln_index_h
 _diffrn_standard_refln_index_k
 _diffrn_standard_refln_index_l
  1 1 1

#=======================================================================

# REFINEMENT DATA

_refine_special_details
;
Substitutionally disordered fluoride and oxide ions were constrained
 to have the same ADP.
;

_reflns_number_total                     82
_reflns_number_gt                        81
_reflns_threshold_expression             I>2σ(I)

_refine_ls_structure_factor_coef         Fsqd
_refine_ls_matrix_type                   full
_refine_ls_R_factor_gt                   0.0123
_refine_ls_wR_factor_gt                  0.0455
_refine_ls_R_factor_all                  0.0123
_refine_ls_wR_factor_ref                 0.0455
_refine_ls_goodness_of_fit_ref           1.13
_refine_ls_goodness_of_fit_gt            1.14
_refine_ls_number_reflns                 82
_refine_ls_number_parameters             6
_refine_ls_number_restraints             0
_refine_ls_number_constraints            2
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(I)+0.0011048977I²)'
_refine_ls_hydrogen_treatment            .
_refine_ls_shift/su_max                  0.0000
_refine_ls_shift/su_mean                 0.0000
_refine_diff_density_max                 0.35
_refine_diff_density_min                 -0.25
_refine_ls_extinction_method             'SHELXL-2017/1 (Sheldrick, 2015)'
_refine_ls_extinction_coef               6.6(4)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'

loop_
 _atom_type_symbol
 _atom_type_scat_length_neutron
 _atom_type_scat_source
 Ba    5.070 International_Tables_Vol_C
 F     5.654 International_Tables_Vol_C
 Li   -1.900 International_Tables_Vol_C
 O     5.803 International_Tables_Vol_C

_atom_sites_solution_primary             iterative
_atom_sites_solution_secondary           .
_atom_sites_solution_hydrogens           .

_computing_data_collection               'NOMAD (Institut Laue-Langevin, 2016)'
_computing_cell_refinement               'RAFD9 (Filhol, 1988)'
_computing_data_reduction
 'RACER (Lehmann & Larsen, 1974; Wilkinson et al., 1988)'
_computing_structure_solution          'SUPERFLIP (Palatinus & Chapuis, 2007)'
_computing_structure_refinement        'Jana2006 (Petříček et al., 2014)'
_computing_molecular_graphics          'VESTA (Momma & Izumi, 2011)'
_computing_publication_material        'Jana2006 (Petříček et al., 2014)'

#=======================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
 _atom_site_constraints
  Ba1 Ba 0 0 0 Uani 0.00734(7) 1 1 d STP . . .
  Li1 Li 0.5 0.5 0.5 Uani 0.01232(11) 1 1 d STP . . .
  F1 F 0.5 0.5 0 Uani 0.01107(7) 3 0.9333 d STP . 1 .
  O1 O 0.5 0.5 0 Uani 0.01107(7) 3 0.0333 d STP . 2 'U=U(F1)'


#=======================================================================

# MOLECULAR GEOMETRY

loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Ba1 O1 . 1_445 2.8269(2) ?
  Ba1 O1 . 1_455 2.8269(2) ?
  Ba1 O1 . 1_545 2.8269(2) ?
  Ba1 O1 . . 2.8269(2) ?
  Ba1 O1 . 5_544 2.8269(2) ?
  Ba1 O1 . 5_545 2.8269(2) ?
  Ba1 O1 . 5_554 2.8269(2) ?
  Ba1 O1 . 5_555 2.8269(2) ?
  Ba1 O1 . 9_454 2.8269(2) ?
  Ba1 O1 . 9_455 2.8269(2) ?
  Ba1 O1 . 9_554 2.8269(2) ?
  Ba1 O1 . 9_555 2.8269(2) ?
  Li1 F1 . . 1.9989(2) ?
  Li1 F1 . 1_556 1.9989(2) ?
  Li1 F1 . 5_555 1.9989(2) ?
  Li1 F1 . 5_655 1.9989(2) ?
  Li1 F1 . 9_555 1.9989(2) ?
  Li1 F1 . 9_565 1.9989(2) ?
  Li1 O1 . . 1.9989(2) ?
  Li1 O1 . 1_556 1.9989(2) ?
  Li1 O1 . 5_555 1.9989(2) ?
  Li1 O1 . 5_655 1.9989(2) ?
  Li1 O1 . 9_555 1.9989(2) ?
  Li1 O1 . 9_565 1.9989(2) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  O1 Ba1 O1 1_445 . 1_455 90.000(4) ?
  O1 Ba1 O1 1_445 . 1_545 90.000(4) ?
  O1 Ba1 O1 1_445 . . 180 ?
  O1 Ba1 O1 1_445 . 5_544 60.000(2) ?
  O1 Ba1 O1 1_445 . 5_545 60.000(2) ?
  O1 Ba1 O1 1_445 . 5_554 120.000(2) ?
  O1 Ba1 O1 1_445 . 5_555 120.000(2) ?
  O1 Ba1 O1 1_445 . 9_454 60.000(2) ?
  O1 Ba1 O1 1_445 . 9_455 60.000(2) ?
  O1 Ba1 O1 1_445 . 9_554 120.000(2) ?
  O1 Ba1 O1 1_445 . 9_555 120.000(2) ?
  O1 Ba1 O1 1_455 . 1_545 180 ?
  O1 Ba1 O1 1_455 . . 90.000(4) ?
  O1 Ba1 O1 1_455 . 5_544 120.000(2) ?
  O1 Ba1 O1 1_455 . 5_545 120.000(2) ?
  O1 Ba1 O1 1_455 . 5_554 60.000(2) ?
  O1 Ba1 O1 1_455 . 5_555 60.000(2) ?
  O1 Ba1 O1 1_455 . 9_454 60.000(2) ?
  O1 Ba1 O1 1_455 . 9_455 60.000(2) ?
  O1 Ba1 O1 1_455 . 9_554 120.000(2) ?
  O1 Ba1 O1 1_455 . 9_555 120.000(2) ?
  O1 Ba1 O1 1_545 . . 90.000(4) ?
  O1 Ba1 O1 1_545 . 5_544 60.000(2) ?
  O1 Ba1 O1 1_545 . 5_545 60.000(2) ?
  O1 Ba1 O1 1_545 . 5_554 120.000(2) ?
  O1 Ba1 O1 1_545 . 5_555 120.000(2) ?
  O1 Ba1 O1 1_545 . 9_454 120.000(2) ?
  O1 Ba1 O1 1_545 . 9_455 120.000(2) ?
  O1 Ba1 O1 1_545 . 9_554 60.000(2) ?
  O1 Ba1 O1 1_545 . 9_555 60.000(2) ?
  O1 Ba1 O1 . . 5_544 120.000(2) ?
  O1 Ba1 O1 . . 5_545 120.000(2) ?
  O1 Ba1 O1 . . 5_554 60.000(2) ?
  O1 Ba1 O1 . . 5_555 60.000(2) ?
  O1 Ba1 O1 . . 9_454 120.000(2) ?
  O1 Ba1 O1 . . 9_455 120.000(2) ?
  O1 Ba1 O1 . . 9_554 60.000(2) ?
  O1 Ba1 O1 . . 9_555 60.000(2) ?
  O1 Ba1 O1 5_544 . 5_545 90.000(4) ?
  O1 Ba1 O1 5_544 . 5_554 90.000(4) ?
  O1 Ba1 O1 5_544 . 5_555 180 ?
  O1 Ba1 O1 5_544 . 9_454 60.000(2) ?
  O1 Ba1 O1 5_544 . 9_455 120.000(2) ?
  O1 Ba1 O1 5_544 . 9_554 60.000(2) ?
  O1 Ba1 O1 5_544 . 9_555 120.000(2) ?
  O1 Ba1 O1 5_545 . 5_554 180 ?
  O1 Ba1 O1 5_545 . 5_555 90.000(4) ?
  O1 Ba1 O1 5_545 . 9_454 120.000(2) ?
  O1 Ba1 O1 5_545 . 9_455 60.000(2) ?
  O1 Ba1 O1 5_545 . 9_554 120.000(2) ?
  O1 Ba1 O1 5_545 . 9_555 60.000(2) ?
  O1 Ba1 O1 5_554 . 5_555 90.000(4) ?
  O1 Ba1 O1 5_554 . 9_454 60.000(2) ?
  O1 Ba1 O1 5_554 . 9_455 120.000(2) ?
  O1 Ba1 O1 5_554 . 9_554 60.000(2) ?
  O1 Ba1 O1 5_554 . 9_555 120.000(2) ?
  O1 Ba1 O1 5_555 . 9_454 120.000(2) ?
  O1 Ba1 O1 5_555 . 9_455 60.000(2) ?
  O1 Ba1 O1 5_555 . 9_554 120.000(2) ?
  O1 Ba1 O1 5_555 . 9_555 60.000(2) ?
  O1 Ba1 O1 9_454 . 9_455 90.000(4) ?
  O1 Ba1 O1 9_454 . 9_554 90.000(4) ?
  O1 Ba1 O1 9_454 . 9_555 180 ?
  O1 Ba1 O1 9_455 . 9_554 180 ?
  O1 Ba1 O1 9_455 . 9_555 90.000(4) ?
  O1 Ba1 O1 9_554 . 9_555 90.000(4) ?
  F1 Li1 F1 . . 1_556 180 ?
  F1 Li1 F1 . . 5_555 90 ?
  F1 Li1 F1 . . 5_655 90 ?
  F1 Li1 F1 . . 9_555 90 ?
  F1 Li1 F1 . . 9_565 90 ?
  F1 Li1 F1 1_556 . 5_555 90 ?
  F1 Li1 F1 1_556 . 5_655 90 ?
  F1 Li1 F1 1_556 . 9_555 90 ?
  F1 Li1 F1 1_556 . 9_565 90 ?
  F1 Li1 F1 5_555 . 5_655 180 ?
  F1 Li1 F1 5_555 . 9_555 90 ?
  F1 Li1 F1 5_555 . 9_565 90 ?
  F1 Li1 F1 5_655 . 9_555 90 ?
  F1 Li1 F1 5_655 . 9_565 90 ?
  F1 Li1 F1 9_555 . 9_565 180 ?
  O1 Li1 O1 . . 1_556 180 ?
  O1 Li1 O1 . . 5_555 90 ?
  O1 Li1 O1 . . 5_655 90 ?
  O1 Li1 O1 . . 9_555 90 ?
  O1 Li1 O1 . . 9_565 90 ?
  O1 Li1 O1 1_556 . 5_555 90 ?
  O1 Li1 O1 1_556 . 5_655 90 ?
  O1 Li1 O1 1_556 . 9_555 90 ?
  O1 Li1 O1 1_556 . 9_565 90 ?
  O1 Li1 O1 5_555 . 5_655 180 ?
  O1 Li1 O1 5_555 . 9_555 90 ?
  O1 Li1 O1 5_555 . 9_565 90 ?
  O1 Li1 O1 5_655 . 9_555 90 ?
  O1 Li1 O1 5_655 . 9_565 90 ?
  O1 Li1 O1 9_555 . 9_565 180 ?

#=======================================================================

# STRUCTURE-FACTOR LIST


#=======================================================================

# REFINEMENT INSTRUCTION FILE


#=======================================================================
data_BaLiF3-412C
#=======================================================================

_database_code_CSD                       434515

# CHEMICAL DATA

_chemical_name_systematic                'barium lithium fluoride oxide'
_chemical_name_structure_type            Perovskite-CaTiO₃
_chemical_formula_iupac                  'Ba Li F2.80 O0.10'
_chemical_formula_sum                    'Ba F2.80 Li O0.10'
_chemical_formula_weight                 199.1
_chemical_compound_source                synthetic

#=======================================================================

# CRYSTAL DATA

_symmetry_cell_setting                   cubic
_symmetry_space_group_name_H-M           'P m -3 m'
_symmetry_space_group_name_Hall          '-P 4 2 3'
_symmetry_Int_Tables_number              221
loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -x,-y,z
 3   -x,y,-z
 4   x,-y,-z
 5   z,x,y
 6   z,-x,-y
 7   -z,-x,y
 8   -z,x,-y
 9   y,z,x
 10  -y,z,-x
 11  y,-z,-x
 12  -y,-z,x
 13  y,x,-z
 14  -y,-x,-z
 15  y,-x,z
 16  -y,x,z
 17  x,z,-y
 18  -x,z,y
 19  -x,-z,-y
 20  x,-z,y
 21  z,y,-x
 22  z,-y,x
 23  -z,y,x
 24  -z,-y,-x
 25  -x,-y,-z
 26  x,y,-z
 27  x,-y,z
 28  -x,y,z
 29  -z,-x,-y
 30  -z,x,y
 31  z,x,-y
 32  z,-x,y
 33  -y,-z,-x
 34  y,-z,x
 35  -y,z,x
 36  y,z,-x
 37  -y,-x,z
 38  y,x,z
 39  -y,x,-z
 40  y,-x,-z
 41  -x,-z,y
 42  x,-z,-y
 43  x,z,y
 44  -x,z,-y
 45  -z,-y,x
 46  -z,y,-x
 47  z,-y,-x
 48  z,y,x

_cell_length_a                           4.0406(2)
_cell_length_b                           4.0406(2)
_cell_length_c                           4.0406(2)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        90
_cell_volume                             65.969(10)
_cell_formula_units_Z                    1

_cell_measurement_reflns_used            120
_cell_measurement_theta_min              6.03
_cell_measurement_theta_max              48.45
_cell_measurement_temperature            685(3)

_exptl_crystal_density_diffrn            5.0111
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            'not measured'
_exptl_crystal_F_000                     19.582

_exptl_absorpt_coefficient_mu            0.051
_exptl_crystal_description               cube
_exptl_crystal_size_max                  5.00
_exptl_crystal_size_mid                  5.00
_exptl_crystal_size_min                  5.00
_exptl_crystal_colour                    colourless
_exptl_absorpt_correction_type           gaussian
_exptl_absorpt_process_details
'Jana2006 (Petříček et al., 2014)'
_exptl_absorpt_correction_T_min          0.9754
_exptl_absorpt_correction_T_max          0.9784

loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 1  0  0  0.25
-1  0  0  0.25
 0  1  0  0.25
 0 -1  0  0.25
 0  0  1  0.25
 0  0 -1  0.25

#=======================================================================

# EXPERIMENTAL DATA

_diffrn_ambient_temperature              685(3)
_diffrn_ambient_environment              vacuum
_diffrn_source                           'nuclear reactor'
_diffrn_source_type                      'ILL high-flux reactor, beam H3'
_diffrn_source_size                      '0.6 \\times 0.6 cm^2^'
_diffrn_source_take-off_angle            56.30
_diffrn_radiation_probe                  neutron
_diffrn_radiation_type                   neutron
_diffrn_radiation_wavelength             0.83860
_diffrn_radiation_monochromator          'Cu 220'
_diffrn_radiation_filter_edge            0.425
_diffrn_measurement_device               'four-circle diffractometer'
_diffrn_measurement_device_type
'D9 position-sensitive detector diffractometer'
_diffrn_measurement_device_details
;
 Eulerian cradle with offset χ circle
;
_diffrn_detector                         '^3^He counter'
_diffrn_detector_type                    'ILL bidim 64mm'
_diffrn_detector_details
;
area detector with pixel size: 2 × 2 mm², 0.25° × 0.25°; pixel
 count: 32 × 32, sensitive area: 64 × 64 mm²
;
_diffrn_detector_area_resol_mean         0.5
_diffrn_measurement_method               'ω and ω-2θ scans'
_diffrn_measurement_specimen_support
;
titanium pin with high-temperature alumina-filled ceramic adhesive
 (Ceramabond 552)
;

_diffrn_reflns_number                    286
_diffrn_reflns_theta_min                 5.96
_diffrn_reflns_theta_max                 49.691
_diffrn_reflns_theta_full                49.691
_diffrn_measured_fraction_theta_max      1.00
_diffrn_measured_fraction_theta_full     1.00
_diffrn_reflns_av_R_equivalents          0.0202
_diffrn_reflns_av_unetI/netI             0.0058
_diffrn_reflns_limit_h_min               0
_diffrn_reflns_limit_h_max               7
_diffrn_reflns_limit_k_min               0
_diffrn_reflns_limit_k_max               7
_diffrn_reflns_limit_l_min               0
_diffrn_reflns_limit_l_max               7

_diffrn_standards_number                 1
_diffrn_standards_interval_count         80
_diffrn_standards_decay_%                -0.1(3)

loop_
 _diffrn_standard_refln_index_h
 _diffrn_standard_refln_index_k
 _diffrn_standard_refln_index_l
  1 1 1

#=======================================================================

# REFINEMENT DATA

_refine_special_details
;
Substitutionally disordered fluoride and oxide ions were constrained
 to have the same ADP.
;

_reflns_number_total                     68
_reflns_number_gt                        67
_reflns_threshold_expression             I>2σ(I)

_refine_ls_structure_factor_coef         Fsqd
_refine_ls_matrix_type                   full
_refine_ls_R_factor_gt                   0.0114
_refine_ls_wR_factor_gt                  0.0383
_refine_ls_R_factor_all                  0.0114
_refine_ls_wR_factor_ref                 0.0383
_refine_ls_goodness_of_fit_ref           0.85
_refine_ls_goodness_of_fit_gt            0.86
_refine_ls_number_reflns                 68
_refine_ls_number_parameters             7
_refine_ls_number_restraints             0
_refine_ls_number_constraints            3
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(I)+0.0013075456I²)'
_refine_ls_hydrogen_treatment            .
_refine_ls_shift/su_max                  0.0000
_refine_ls_shift/su_mean                 0.0000
_refine_diff_density_max                 0.13
_refine_diff_density_min                 -0.12
_refine_ls_extinction_method             'SHELXL-2017/1 (Sheldrick, 2015)'
_refine_ls_extinction_coef               5.0(3)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'

loop_
 _atom_type_symbol
 _atom_type_scat_length_neutron
 _atom_type_scat_source
 Ba    5.070 International_Tables_Vol_C
 F     5.654 International_Tables_Vol_C
 Li   -1.900 International_Tables_Vol_C
 O     5.803 International_Tables_Vol_C

_atom_sites_solution_primary             iterative
_atom_sites_solution_secondary           .
_atom_sites_solution_hydrogens           .

_computing_data_collection               'NOMAD (Institut Laue-Langevin, 2016)'
_computing_cell_refinement               'RAFD9 (Filhol, 1988)'
_computing_data_reduction
 'RACER (Lehmann & Larsen, 1974; Wilkinson et al., 1988)'
_computing_structure_solution          'SUPERFLIP (Palatinus & Chapuis, 2007)'
_computing_structure_refinement        'Jana2006 (Petříček et al., 2014)'
_computing_molecular_graphics          'VESTA (Momma & Izumi, 2011)'
_computing_publication_material        'Jana2006 (Petříček et al., 2014)'

#=======================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
 _atom_site_constraints
  Ba1 Ba 0 0 0 Uani 0.01899(9) 1 1 d STP . . .
  Li1 Li 0.5 0.5 0.5 Uani 0.02730(18) 1 1 d STP . . .
  F1 F 0.5 0.5 0 Uani 0.02823(12) 3 0.9333 d STP . 1 .
  O1 O 0.5 0.5 0 Uani 0.02823(12) 3 0.0333 d STP . 2 'U=U(F1)'


loop_
 _jana_atom_site_ADP_C_label
 _jana_atom_site_ADP_C_type_symbol
 _jana_atom_site_ADP_C_111
 _jana_atom_site_ADP_C_112
 _jana_atom_site_ADP_C_113
 _jana_atom_site_ADP_C_122
 _jana_atom_site_ADP_C_123
 _jana_atom_site_ADP_C_133
 _jana_atom_site_ADP_C_222
 _jana_atom_site_ADP_C_223
 _jana_atom_site_ADP_C_233
 _jana_atom_site_ADP_C_333
 F1 F 0 0 0 0 0 0 0 0 0 0
 O1 O 0 0 0 0 0 0 0 0 0 0

loop_
 _jana_atom_site_ADP_D_label
 _jana_atom_site_ADP_D_type_symbol
 _jana_atom_site_ADP_D_1111
 _jana_atom_site_ADP_D_1112
 _jana_atom_site_ADP_D_1113
 _jana_atom_site_ADP_D_1122
 _jana_atom_site_ADP_D_1123
 _jana_atom_site_ADP_D_1133
 _jana_atom_site_ADP_D_1222
 _jana_atom_site_ADP_D_1223
 _jana_atom_site_ADP_D_1233
 _jana_atom_site_ADP_D_1333
 _jana_atom_site_ADP_D_2222
 _jana_atom_site_ADP_D_2223
 _jana_atom_site_ADP_D_2233
 _jana_atom_site_ADP_D_2333
 _jana_atom_site_ADP_D_3333
 F1 F 0.0044(14) 0 0 0 0 0 0 0 0 0 0.0044(14) 0 0 0 0
 O1 O 0.0044(14) 0 0 0 0 0 0 0 0 0 0.0044(14) 0 0 0 0

#=======================================================================

# MOLECULAR GEOMETRY

loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Ba1 O1 . 1_445 2.8571(2) ?
  Ba1 O1 . 1_455 2.8571(2) ?
  Ba1 O1 . 1_545 2.8571(2) ?
  Ba1 O1 . . 2.8571(2) ?
  Ba1 O1 . 5_544 2.8571(2) ?
  Ba1 O1 . 5_545 2.8571(2) ?
  Ba1 O1 . 5_554 2.8571(2) ?
  Ba1 O1 . 5_555 2.8571(2) ?
  Ba1 O1 . 9_454 2.8571(2) ?
  Ba1 O1 . 9_455 2.8571(2) ?
  Ba1 O1 . 9_554 2.8571(2) ?
  Ba1 O1 . 9_555 2.8571(2) ?
  Li1 F1 . . 2.0203(2) ?
  Li1 F1 . 1_556 2.0203(2) ?
  Li1 F1 . 5_555 2.0203(2) ?
  Li1 F1 . 5_655 2.0203(2) ?
  Li1 F1 . 9_555 2.0203(2) ?
  Li1 F1 . 9_565 2.0203(2) ?
  Li1 O1 . . 2.0203(2) ?
  Li1 O1 . 1_556 2.0203(2) ?
  Li1 O1 . 5_555 2.0203(2) ?
  Li1 O1 . 5_655 2.0203(2) ?
  Li1 O1 . 9_555 2.0203(2) ?
  Li1 O1 . 9_565 2.0203(2) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  O1 Ba1 O1 1_445 . 1_455 90.000(4) ?
  O1 Ba1 O1 1_445 . 1_545 90.000(4) ?
  O1 Ba1 O1 1_445 . . 180 ?
  O1 Ba1 O1 1_445 . 5_544 60.000(2) ?
  O1 Ba1 O1 1_445 . 5_545 60.000(2) ?
  O1 Ba1 O1 1_445 . 5_554 120.000(2) ?
  O1 Ba1 O1 1_445 . 5_555 120.000(2) ?
  O1 Ba1 O1 1_445 . 9_454 60.000(2) ?
  O1 Ba1 O1 1_445 . 9_455 60.000(2) ?
  O1 Ba1 O1 1_445 . 9_554 120.000(2) ?
  O1 Ba1 O1 1_445 . 9_555 120.000(2) ?
  O1 Ba1 O1 1_455 . 1_545 180 ?
  O1 Ba1 O1 1_455 . . 90.000(4) ?
  O1 Ba1 O1 1_455 . 5_544 120.000(2) ?
  O1 Ba1 O1 1_455 . 5_545 120.000(2) ?
  O1 Ba1 O1 1_455 . 5_554 60.000(2) ?
  O1 Ba1 O1 1_455 . 5_555 60.000(2) ?
  O1 Ba1 O1 1_455 . 9_454 60.000(2) ?
  O1 Ba1 O1 1_455 . 9_455 60.000(2) ?
  O1 Ba1 O1 1_455 . 9_554 120.000(2) ?
  O1 Ba1 O1 1_455 . 9_555 120.000(2) ?
  O1 Ba1 O1 1_545 . . 90.000(4) ?
  O1 Ba1 O1 1_545 . 5_544 60.000(2) ?
  O1 Ba1 O1 1_545 . 5_545 60.000(2) ?
  O1 Ba1 O1 1_545 . 5_554 120.000(2) ?
  O1 Ba1 O1 1_545 . 5_555 120.000(2) ?
  O1 Ba1 O1 1_545 . 9_454 120.000(2) ?
  O1 Ba1 O1 1_545 . 9_455 120.000(2) ?
  O1 Ba1 O1 1_545 . 9_554 60.000(2) ?
  O1 Ba1 O1 1_545 . 9_555 60.000(2) ?
  O1 Ba1 O1 . . 5_544 120.000(2) ?
  O1 Ba1 O1 . . 5_545 120.000(2) ?
  O1 Ba1 O1 . . 5_554 60.000(2) ?
  O1 Ba1 O1 . . 5_555 60.000(2) ?
  O1 Ba1 O1 . . 9_454 120.000(2) ?
  O1 Ba1 O1 . . 9_455 120.000(2) ?
  O1 Ba1 O1 . . 9_554 60.000(2) ?
  O1 Ba1 O1 . . 9_555 60.000(2) ?
  O1 Ba1 O1 5_544 . 5_545 90.000(4) ?
  O1 Ba1 O1 5_544 . 5_554 90.000(4) ?
  O1 Ba1 O1 5_544 . 5_555 180 ?
  O1 Ba1 O1 5_544 . 9_454 60.000(2) ?
  O1 Ba1 O1 5_544 . 9_455 120.000(2) ?
  O1 Ba1 O1 5_544 . 9_554 60.000(2) ?
  O1 Ba1 O1 5_544 . 9_555 120.000(2) ?
  O1 Ba1 O1 5_545 . 5_554 180 ?
  O1 Ba1 O1 5_545 . 5_555 90.000(4) ?
  O1 Ba1 O1 5_545 . 9_454 120.000(2) ?
  O1 Ba1 O1 5_545 . 9_455 60.000(2) ?
  O1 Ba1 O1 5_545 . 9_554 120.000(2) ?
  O1 Ba1 O1 5_545 . 9_555 60.000(2) ?
  O1 Ba1 O1 5_554 . 5_555 90.000(4) ?
  O1 Ba1 O1 5_554 . 9_454 60.000(2) ?
  O1 Ba1 O1 5_554 . 9_455 120.000(2) ?
  O1 Ba1 O1 5_554 . 9_554 60.000(2) ?
  O1 Ba1 O1 5_554 . 9_555 120.000(2) ?
  O1 Ba1 O1 5_555 . 9_454 120.000(2) ?
  O1 Ba1 O1 5_555 . 9_455 60.000(2) ?
  O1 Ba1 O1 5_555 . 9_554 120.000(2) ?
  O1 Ba1 O1 5_555 . 9_555 60.000(2) ?
  O1 Ba1 O1 9_454 . 9_455 90.000(4) ?
  O1 Ba1 O1 9_454 . 9_554 90.000(4) ?
  O1 Ba1 O1 9_454 . 9_555 180 ?
  O1 Ba1 O1 9_455 . 9_554 180 ?
  O1 Ba1 O1 9_455 . 9_555 90.000(4) ?
  O1 Ba1 O1 9_554 . 9_555 90.000(4) ?
  F1 Li1 F1 . . 1_556 180 ?
  F1 Li1 F1 . . 5_555 90 ?
  F1 Li1 F1 . . 5_655 90 ?
  F1 Li1 F1 . . 9_555 90 ?
  F1 Li1 F1 . . 9_565 90 ?
  F1 Li1 O1 . . . 0 ?
  F1 Li1 O1 . . 1_556 180 ?
  F1 Li1 O1 . . 5_555 90 ?
  F1 Li1 O1 . . 5_655 90 ?
  F1 Li1 O1 . . 9_555 90 ?
  F1 Li1 O1 . . 9_565 90 ?
  F1 Li1 F1 1_556 . 5_555 90 ?
  F1 Li1 F1 1_556 . 5_655 90 ?
  F1 Li1 F1 1_556 . 9_555 90 ?
  F1 Li1 F1 1_556 . 9_565 90 ?
  F1 Li1 O1 1_556 . . 180 ?
  F1 Li1 O1 1_556 . 1_556 0 ?
  F1 Li1 O1 1_556 . 5_555 90 ?
  F1 Li1 O1 1_556 . 5_655 90 ?
  F1 Li1 O1 1_556 . 9_555 90 ?
  F1 Li1 O1 1_556 . 9_565 90 ?
  F1 Li1 F1 5_555 . 5_655 180 ?
  F1 Li1 F1 5_555 . 9_555 90 ?
  F1 Li1 F1 5_555 . 9_565 90 ?
  F1 Li1 O1 5_555 . . 90 ?
  F1 Li1 O1 5_555 . 1_556 90 ?
  F1 Li1 O1 5_555 . 5_555 0 ?
  F1 Li1 O1 5_555 . 5_655 180 ?
  F1 Li1 O1 5_555 . 9_555 90 ?
  F1 Li1 O1 5_555 . 9_565 90 ?
  F1 Li1 F1 5_655 . 9_555 90 ?
  F1 Li1 F1 5_655 . 9_565 90 ?
  F1 Li1 O1 5_655 . . 90 ?
  F1 Li1 O1 5_655 . 1_556 90 ?
  F1 Li1 O1 5_655 . 5_555 180 ?
  F1 Li1 O1 5_655 . 5_655 0 ?
  F1 Li1 O1 5_655 . 9_555 90 ?
  F1 Li1 O1 5_655 . 9_565 90 ?
  F1 Li1 F1 9_555 . 9_565 180 ?
  F1 Li1 O1 9_555 . . 90 ?
  F1 Li1 O1 9_555 . 1_556 90 ?
  F1 Li1 O1 9_555 . 5_555 90 ?
  F1 Li1 O1 9_555 . 5_655 90 ?
  F1 Li1 O1 9_555 . 9_555 0 ?
  F1 Li1 O1 9_555 . 9_565 180 ?
  F1 Li1 O1 9_565 . . 90 ?
  F1 Li1 O1 9_565 . 1_556 90 ?
  F1 Li1 O1 9_565 . 5_555 90 ?
  F1 Li1 O1 9_565 . 5_655 90 ?
  F1 Li1 O1 9_565 . 9_555 180 ?
  F1 Li1 O1 9_565 . 9_565 0 ?
  O1 Li1 O1 . . 1_556 180 ?
  O1 Li1 O1 . . 5_555 90 ?
  O1 Li1 O1 . . 5_655 90 ?
  O1 Li1 O1 . . 9_555 90 ?
  O1 Li1 O1 . . 9_565 90 ?
  O1 Li1 O1 1_556 . 5_555 90 ?
  O1 Li1 O1 1_556 . 5_655 90 ?
  O1 Li1 O1 1_556 . 9_555 90 ?
  O1 Li1 O1 1_556 . 9_565 90 ?
  O1 Li1 O1 5_555 . 5_655 180 ?
  O1 Li1 O1 5_555 . 9_555 90 ?
  O1 Li1 O1 5_555 . 9_565 90 ?
  O1 Li1 O1 5_655 . 9_555 90 ?
  O1 Li1 O1 5_655 . 9_565 90 ?
  O1 Li1 O1 9_555 . 9_565 180 ?

#=======================================================================

# STRUCTURE-FACTOR LIST


#=======================================================================

# REFINEMENT INSTRUCTION FILE


#=======================================================================
data_BaLiF3-555C
#=======================================================================

_database_code_CSD                       434516

# CHEMICAL DATA

_chemical_name_systematic                'barium lithium fluoride oxide'
_chemical_name_structure_type            Perovskite-CaTiO₃
_chemical_formula_iupac                  'Ba Li F2.80 O0.10'
_chemical_formula_sum                    'Ba F2.80 Li O0.10'
_chemical_formula_weight                 199.1
_chemical_compound_source                synthetic

#=======================================================================

# CRYSTAL DATA

_symmetry_cell_setting                   cubic
_symmetry_space_group_name_H-M           'P m -3 m'
_symmetry_space_group_name_Hall          '-P 4 2 3'
_symmetry_Int_Tables_number              221


loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -x,-y,z
 3   -x,y,-z
 4   x,-y,-z
 5   z,x,y
 6   z,-x,-y
 7   -z,-x,y
 8   -z,x,-y
 9   y,z,x
 10  -y,z,-x
 11  y,-z,-x
 12  -y,-z,x
 13  y,x,-z
 14  -y,-x,-z
 15  y,-x,z
 16  -y,x,z
 17  x,z,-y
 18  -x,z,y
 19  -x,-z,-y
 20  x,-z,y
 21  z,y,-x
 22  z,-y,x
 23  -z,y,x
 24  -z,-y,-x
 25  -x,-y,-z
 26  x,y,-z
 27  x,-y,z
 28  -x,y,z
 29  -z,-x,-y
 30  -z,x,y
 31  z,x,-y
 32  z,-x,y
 33  -y,-z,-x
 34  y,-z,x
 35  -y,z,x
 36  y,z,-x
 37  -y,-x,z
 38  y,x,z
 39  -y,x,-z
 40  y,-x,-z
 41  -x,-z,y
 42  x,-z,-y
 43  x,z,y
 44  -x,z,-y
 45  -z,-y,x
 46  -z,y,-x
 47  z,-y,-x
 48  z,y,x

_cell_length_a                           4.0581(3)
_cell_length_b                           4.0581(3)
_cell_length_c                           4.0581(3)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        90
_cell_volume                             66.830(15)
_cell_formula_units_Z                    1

_cell_measurement_reflns_used            103
_cell_measurement_theta_min              5.96
_cell_measurement_theta_max              43.29
_cell_measurement_temperature            827(3)

_exptl_crystal_density_diffrn            4.9465
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            'not measured'
_exptl_crystal_F_000                     19.582

_exptl_absorpt_coefficient_mu            0.050
_exptl_crystal_description               cube
_exptl_crystal_size_max                  5.00
_exptl_crystal_size_mid                  5.00
_exptl_crystal_size_min                  5.00
_exptl_crystal_colour                    colourless
_exptl_absorpt_correction_type           gaussian
_exptl_absorpt_process_details
'Jana2006 (Petříček et al., 2014)'
_exptl_absorpt_correction_T_min          0.9757
_exptl_absorpt_correction_T_max          0.9787

loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 1  0  0  0.25
-1  0  0  0.25
 0  1  0  0.25
 0 -1  0  0.25
 0  0  1  0.25
 0  0 -1  0.25

#=======================================================================

# EXPERIMENTAL DATA

_diffrn_ambient_temperature              827(3)
_diffrn_ambient_environment              vacuum
_diffrn_source                           'nuclear reactor'
_diffrn_source_type                      'ILL high-flux reactor, beam H3'
_diffrn_source_size                      '0.6 \\times 0.6 cm^2^'
_diffrn_source_take-off_angle            56.30
_diffrn_radiation_probe                  neutron
_diffrn_radiation_type                   neutron
_diffrn_radiation_wavelength             0.83860
_diffrn_radiation_monochromator          'Cu 220'
_diffrn_radiation_filter_edge            0.425
_diffrn_measurement_device               'four-circle diffractometer'
_diffrn_measurement_device_type
'D9 position-sensitive detector diffractometer'
_diffrn_measurement_device_details
;
 Eulerian cradle with offset χ circle
;
_diffrn_detector                         '^3^He counter'
_diffrn_detector_type                    'ILL bidim 64mm'
_diffrn_detector_details
;
area detector with pixel size: 2 × 2 mm², 0.25° × 0.25°; pixel
 count: 32 × 32, sensitive area: 64 × 64 mm²
;
_diffrn_detector_area_resol_mean         0.5
_diffrn_measurement_method               'ω and ω-2θ scans'
_diffrn_measurement_specimen_support
;
titanium pin with high-temperature alumina-filled ceramic adhesive
 (Ceramabond 552)
;

_diffrn_reflns_number                    362
_diffrn_reflns_theta_min                 5.93
_diffrn_reflns_theta_max                 56.42
_diffrn_reflns_theta_full                56.42
_diffrn_measured_fraction_theta_max      1.00
_diffrn_measured_fraction_theta_full     1.00
_diffrn_reflns_av_R_equivalents          0.0232
_diffrn_reflns_av_unetI/netI             0.0065
_diffrn_reflns_limit_h_min               -4
_diffrn_reflns_limit_h_max               8
_diffrn_reflns_limit_k_min               -4
_diffrn_reflns_limit_k_max               8
_diffrn_reflns_limit_l_min               0
_diffrn_reflns_limit_l_max               8

_diffrn_standards_number                 1
_diffrn_standards_interval_count         80
_diffrn_standards_decay_%                -0.06(19)

loop_
 _diffrn_standard_refln_index_h
 _diffrn_standard_refln_index_k
 _diffrn_standard_refln_index_l
  1 1 1

#=======================================================================

# REFINEMENT DATA

_refine_special_details
;
Substitutionally disordered fluoride and oxide ions were constrained
 to have the same ADP.
;
_reflns_number_total                     82
_reflns_number_gt                        74
_reflns_threshold_expression             I>2σ(I)

_refine_ls_structure_factor_coef         Fsqd
_refine_ls_matrix_type                   full
_refine_ls_R_factor_gt                   0.0154
_refine_ls_wR_factor_gt                  0.0513
_refine_ls_R_factor_all                  0.0189
_refine_ls_wR_factor_ref                 0.0540
_refine_ls_goodness_of_fit_ref           1.02
_refine_ls_goodness_of_fit_gt            1.02
_refine_ls_number_reflns                 82
_refine_ls_number_parameters             7
_refine_ls_number_restraints             0
_refine_ls_number_constraints            3
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(I)+0.0015539365I²)'
_refine_ls_hydrogen_treatment            .
_refine_ls_shift/su_max                  0.0000
_refine_ls_shift/su_mean                 0.0000
_refine_diff_density_max                 0.12
_refine_diff_density_min                 -0.20
_refine_ls_extinction_method             'SHELXL-2017/1 (Sheldrick, 2015)'
_refine_ls_extinction_coef               5.3(4)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'

loop_
 _atom_type_symbol
 _atom_type_scat_length_neutron
 _atom_type_scat_source
 Ba    5.070 International_Tables_Vol_C
 F     5.654 International_Tables_Vol_C
 Li   -1.900 International_Tables_Vol_C
 O     5.803 International_Tables_Vol_C

_atom_sites_solution_primary             iterative
_atom_sites_solution_secondary           .
_atom_sites_solution_hydrogens           .

_computing_data_collection               'NOMAD (Institut Laue-Langevin, 2016)'
_computing_cell_refinement               'RAFD9 (Filhol, 1988)'
_computing_data_reduction
 'RACER (Lehmann & Larsen, 1974; Wilkinson et al., 1988)'
_computing_structure_solution          'SUPERFLIP (Palatinus & Chapuis, 2007)'
_computing_structure_refinement        'Jana2006 (Petříček et al., 2014)'
_computing_molecular_graphics          'VESTA (Momma & Izumi, 2011)'
_computing_publication_material        'Jana2006 (Petříček et al., 2014)'

#=======================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
 _atom_site_constraints
  Ba1 Ba 0 0 0 Uani 0.02452(11) 1 1 d STP . . .
  Li1 Li 0.5 0.5 0.5 Uani 0.0342(2) 1 1 d STP . . .
  F1 F 0.5 0.5 0 Uani 0.03558(15) 3 0.9333 d STP . 1 .
  O1 O 0.5 0.5 0 Uani 0.03558(15) 3 0.0333 d STP . 2 'U=U(F1)'


loop_
 _jana_atom_site_ADP_C_label
 _jana_atom_site_ADP_C_type_symbol
 _jana_atom_site_ADP_C_111
 _jana_atom_site_ADP_C_112
 _jana_atom_site_ADP_C_113
 _jana_atom_site_ADP_C_122
 _jana_atom_site_ADP_C_123
 _jana_atom_site_ADP_C_133
 _jana_atom_site_ADP_C_222
 _jana_atom_site_ADP_C_223
 _jana_atom_site_ADP_C_233
 _jana_atom_site_ADP_C_333
 F1 F 0 0 0 0 0 0 0 0 0 0
 O1 O 0 0 0 0 0 0 0 0 0 0

loop_
 _jana_atom_site_ADP_D_label
 _jana_atom_site_ADP_D_type_symbol
 _jana_atom_site_ADP_D_1111
 _jana_atom_site_ADP_D_1112
 _jana_atom_site_ADP_D_1113
 _jana_atom_site_ADP_D_1122
 _jana_atom_site_ADP_D_1123
 _jana_atom_site_ADP_D_1133
 _jana_atom_site_ADP_D_1222
 _jana_atom_site_ADP_D_1223
 _jana_atom_site_ADP_D_1233
 _jana_atom_site_ADP_D_1333
 _jana_atom_site_ADP_D_2222
 _jana_atom_site_ADP_D_2223
 _jana_atom_site_ADP_D_2233
 _jana_atom_site_ADP_D_2333
 _jana_atom_site_ADP_D_3333
 F1 F 0 0 0 0 0 0 0 0 0 0 0 0 0 0 -0.0069(15)
 O1 O 0 0 0 0 0 0 0 0 0 0 0 0 0 0 -0.0069(15)

#=======================================================================

# MOLECULAR GEOMETRY

loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Ba1 O1 . 1_445 2.8695(3) ?
  Ba1 O1 . 1_455 2.8695(3) ?
  Ba1 O1 . 1_545 2.8695(3) ?
  Ba1 O1 . . 2.8695(3) ?
  Ba1 O1 . 5_544 2.8695(3) ?
  Ba1 O1 . 5_545 2.8695(3) ?
  Ba1 O1 . 5_554 2.8695(3) ?
  Ba1 O1 . 5_555 2.8695(3) ?
  Ba1 O1 . 9_454 2.8695(3) ?
  Ba1 O1 . 9_455 2.8695(3) ?
  Ba1 O1 . 9_554 2.8695(3) ?
  Ba1 O1 . 9_555 2.8695(3) ?
  Li1 O1 . . 2.0291(3) ?
  Li1 O1 . 1_556 2.0291(3) ?
  Li1 O1 . 5_555 2.0291(3) ?
  Li1 O1 . 5_655 2.0291(3) ?
  Li1 O1 . 9_555 2.0291(3) ?
  Li1 O1 . 9_565 2.0291(3) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  O1 Ba1 O1 1_445 . 1_455 90.000(6) ?
  O1 Ba1 O1 1_445 . 1_545 90.000(6) ?
  O1 Ba1 O1 1_445 . . 180 ?
  O1 Ba1 O1 1_445 . 5_544 60.000(3) ?
  O1 Ba1 O1 1_445 . 5_545 60.000(3) ?
  O1 Ba1 O1 1_445 . 5_554 120.000(3) ?
  O1 Ba1 O1 1_445 . 5_555 120.000(3) ?
  O1 Ba1 O1 1_445 . 9_454 60.000(3) ?
  O1 Ba1 O1 1_445 . 9_455 60.000(3) ?
  O1 Ba1 O1 1_445 . 9_554 120.000(3) ?
  O1 Ba1 O1 1_445 . 9_555 120.000(3) ?
  O1 Ba1 O1 1_455 . 1_545 180 ?
  O1 Ba1 O1 1_455 . . 90.000(6) ?
  O1 Ba1 O1 1_455 . 5_544 120.000(3) ?
  O1 Ba1 O1 1_455 . 5_545 120.000(3) ?
  O1 Ba1 O1 1_455 . 5_554 60.000(3) ?
  O1 Ba1 O1 1_455 . 5_555 60.000(3) ?
  O1 Ba1 O1 1_455 . 9_454 60.000(3) ?
  O1 Ba1 O1 1_455 . 9_455 60.000(3) ?
  O1 Ba1 O1 1_455 . 9_554 120.000(3) ?
  O1 Ba1 O1 1_455 . 9_555 120.000(3) ?
  O1 Ba1 O1 1_545 . . 90.000(6) ?
  O1 Ba1 O1 1_545 . 5_544 60.000(3) ?
  O1 Ba1 O1 1_545 . 5_545 60.000(3) ?
  O1 Ba1 O1 1_545 . 5_554 120.000(3) ?
  O1 Ba1 O1 1_545 . 5_555 120.000(3) ?
  O1 Ba1 O1 1_545 . 9_454 120.000(3) ?
  O1 Ba1 O1 1_545 . 9_455 120.000(3) ?
  O1 Ba1 O1 1_545 . 9_554 60.000(3) ?
  O1 Ba1 O1 1_545 . 9_555 60.000(3) ?
  O1 Ba1 O1 . . 5_544 120.000(3) ?
  O1 Ba1 O1 . . 5_545 120.000(3) ?
  O1 Ba1 O1 . . 5_554 60.000(3) ?
  O1 Ba1 O1 . . 5_555 60.000(3) ?
  O1 Ba1 O1 . . 9_454 120.000(3) ?
  O1 Ba1 O1 . . 9_455 120.000(3) ?
  O1 Ba1 O1 . . 9_554 60.000(3) ?
  O1 Ba1 O1 . . 9_555 60.000(3) ?
  O1 Ba1 O1 5_544 . 5_545 90.000(6) ?
  O1 Ba1 O1 5_544 . 5_554 90.000(6) ?
  O1 Ba1 O1 5_544 . 5_555 180 ?
  O1 Ba1 O1 5_544 . 9_454 60.000(3) ?
  O1 Ba1 O1 5_544 . 9_455 120.000(3) ?
  O1 Ba1 O1 5_544 . 9_554 60.000(3) ?
  O1 Ba1 O1 5_544 . 9_555 120.000(3) ?
  O1 Ba1 O1 5_545 . 5_554 180 ?
  O1 Ba1 O1 5_545 . 5_555 90.000(6) ?
  O1 Ba1 O1 5_545 . 9_454 120.000(3) ?
  O1 Ba1 O1 5_545 . 9_455 60.000(3) ?
  O1 Ba1 O1 5_545 . 9_554 120.000(3) ?
  O1 Ba1 O1 5_545 . 9_555 60.000(3) ?
  O1 Ba1 O1 5_554 . 5_555 90.000(6) ?
  O1 Ba1 O1 5_554 . 9_454 60.000(3) ?
  O1 Ba1 O1 5_554 . 9_455 120.000(3) ?
  O1 Ba1 O1 5_554 . 9_554 60.000(3) ?
  O1 Ba1 O1 5_554 . 9_555 120.000(3) ?
  O1 Ba1 O1 5_555 . 9_454 120.000(3) ?
  O1 Ba1 O1 5_555 . 9_455 60.000(3) ?
  O1 Ba1 O1 5_555 . 9_554 120.000(3) ?
  O1 Ba1 O1 5_555 . 9_555 60.000(3) ?
  O1 Ba1 O1 9_454 . 9_455 90.000(6) ?
  O1 Ba1 O1 9_454 . 9_554 90.000(6) ?
  O1 Ba1 O1 9_454 . 9_555 180 ?
  O1 Ba1 O1 9_455 . 9_554 180 ?
  O1 Ba1 O1 9_455 . 9_555 90.000(6) ?
  O1 Ba1 O1 9_554 . 9_555 90.000(6) ?
  O1 Li1 O1 . . 1_556 180 ?
  O1 Li1 O1 . . 5_555 90 ?
  O1 Li1 O1 . . 5_655 90 ?
  O1 Li1 O1 . . 9_555 90 ?
  O1 Li1 O1 . . 9_565 90 ?
  O1 Li1 O1 1_556 . 5_555 90 ?
  O1 Li1 O1 1_556 . 5_655 90 ?
  O1 Li1 O1 1_556 . 9_555 90 ?
  O1 Li1 O1 1_556 . 9_565 90 ?
  O1 Li1 O1 5_555 . 5_655 180 ?
  O1 Li1 O1 5_555 . 9_555 90 ?
  O1 Li1 O1 5_555 . 9_565 90 ?
  O1 Li1 O1 5_655 . 9_555 90 ?
  O1 Li1 O1 5_655 . 9_565 90 ?
  O1 Li1 O1 9_555 . 9_565 180 ?

#=======================================================================

# STRUCTURE-FACTOR LIST


#=======================================================================

# REFINEMENT INSTRUCTION FILE


#=======================================================================
data_BaLiF3-636C
#=======================================================================

_database_code_CSD                       434517

# CHEMICAL DATA

_chemical_name_systematic                'barium lithium fluoride oxide'
_chemical_name_structure_type            Perovskite-CaTiO₃
_chemical_formula_iupac                  'Ba Li F2.80 O0.10'
_chemical_formula_sum                    'Ba F2.80 Li O0.10'
_chemical_formula_weight                 199.1
_chemical_compound_source                synthetic

#=======================================================================

# CRYSTAL DATA

_symmetry_cell_setting                   cubic
_symmetry_space_group_name_H-M           'P m -3 m'
_symmetry_space_group_name_Hall          '-P 4 2 3'
_symmetry_Int_Tables_number              221

loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -x,-y,z
 3   -x,y,-z
 4   x,-y,-z
 5   z,x,y
 6   z,-x,-y
 7   -z,-x,y
 8   -z,x,-y
 9   y,z,x
 10  -y,z,-x
 11  y,-z,-x
 12  -y,-z,x
 13  y,x,-z
 14  -y,-x,-z
 15  y,-x,z
 16  -y,x,z
 17  x,z,-y
 18  -x,z,y
 19  -x,-z,-y
 20  x,-z,y
 21  z,y,-x
 22  z,-y,x
 23  -z,y,x
 24  -z,-y,-x
 25  -x,-y,-z
 26  x,y,-z
 27  x,-y,z
 28  -x,y,z
 29  -z,-x,-y
 30  -z,x,y
 31  z,x,-y
 32  z,-x,y
 33  -y,-z,-x
 34  y,-z,x
 35  -y,z,x
 36  y,z,-x
 37  -y,-x,z
 38  y,x,z
 39  -y,x,-z
 40  y,-x,-z
 41  -x,-z,y
 42  x,-z,-y
 43  x,z,y
 44  -x,z,-y
 45  -z,-y,x
 46  -z,y,-x
 47  z,-y,-x
 48  z,y,x

_cell_length_a                           4.0763(4)
_cell_length_b                           4.0763(4)
_cell_length_c                           4.0763(4)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        90
_cell_volume                             67.73(2)
_cell_formula_units_Z                    1

_cell_measurement_reflns_used            628
_cell_measurement_theta_min              5.92
_cell_measurement_theta_max              47.28
_cell_measurement_temperature            909.4(9)

_exptl_crystal_density_diffrn            4.8805
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            'not measured'
_exptl_crystal_F_000                     19.581

_exptl_crystal_description               cube
_exptl_crystal_size_max                  5.00
_exptl_crystal_size_mid                  5.00
_exptl_crystal_size_min                  5.00
_exptl_crystal_colour                    colourless
_exptl_absorpt_correction_type           gaussian
_exptl_absorpt_process_details
'Jana2006 (Petříček et al., 2014)'
_exptl_absorpt_correction_T_min          0.9760
_exptl_absorpt_correction_T_max          0.9789

loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 1  0  0  0.25
-1  0  0  0.25
 0  1  0  0.25
 0 -1  0  0.25
 0  0  1  0.25
 0  0 -1  0.25

#=======================================================================

# EXPERIMENTAL DATA

_diffrn_ambient_temperature              909.4(9)
_diffrn_ambient_environment              vacuum
_diffrn_source                           'nuclear reactor'
_diffrn_source_type                      'ILL high-flux reactor, beam H3'
_diffrn_source_size                      '0.6 \\times 0.6 cm^2^'
_diffrn_source_take-off_angle            56.30
_diffrn_radiation_probe                  neutron
_diffrn_radiation_type                   neutron
_diffrn_radiation_wavelength             0.83860
_diffrn_radiation_monochromator          'Cu 220'
_diffrn_radiation_filter_edge            0.425
_diffrn_measurement_device               'four-circle diffractometer'
_diffrn_measurement_device_type
'D9 position-sensitive detector diffractometer'
_diffrn_measurement_device_details
;
 Eulerian cradle with offset χ circle
;
_diffrn_detector                         '^3^He counter'
_diffrn_detector_type                    'ILL bidim 64mm'
_diffrn_detector_details
;
area detector with pixel size: 2 × 2 mm², 0.25° × 0.25°; pixel
 count: 32 × 32, sensitive area: 64 × 64 mm²
;
_diffrn_detector_area_resol_mean         0.5
_diffrn_measurement_method               'ω and ω-2θ scans'
_diffrn_measurement_specimen_support
;
titanium pin with high-temperature alumina-filled ceramic adhesive
 (Ceramabond 552)
;

_diffrn_reflns_number                    343
_diffrn_reflns_theta_min                 5.9
_diffrn_reflns_theta_max                 56.03
_diffrn_reflns_theta_full                41.2
_diffrn_measured_fraction_theta_max      0.95
_diffrn_measured_fraction_theta_full     0.98
_diffrn_reflns_av_R_equivalents          0.0212
_diffrn_reflns_av_unetI/netI             0.0068
_diffrn_reflns_limit_h_min               -4
_diffrn_reflns_limit_h_max               8
_diffrn_reflns_limit_k_min               -4
_diffrn_reflns_limit_k_max               8
_diffrn_reflns_limit_l_min               0
_diffrn_reflns_limit_l_max               8

_diffrn_standards_number                 1
_diffrn_standards_interval_count         80
_diffrn_standards_decay_%                -0.7(4)

loop_
 _diffrn_standard_refln_index_h
 _diffrn_standard_refln_index_k
 _diffrn_standard_refln_index_l
  1 1 1

#=======================================================================

# REFINEMENT DATA

_refine_special_details
;
Substitutionally disordered fluoride and oxide ions were constrained
 to have the same ADP.
;

_reflns_number_total                     78
_reflns_number_gt                        70
_reflns_threshold_expression             I>2σ(I)

_refine_ls_structure_factor_coef         Fsqd
_refine_ls_matrix_type                   full
_refine_ls_R_factor_gt                   0.0113
_refine_ls_wR_factor_gt                  0.0410
_refine_ls_R_factor_all                  0.0148
_refine_ls_wR_factor_ref                 0.0450
_refine_ls_goodness_of_fit_ref           0.98
_refine_ls_goodness_of_fit_gt            0.95
_refine_ls_number_reflns                 78
_refine_ls_number_parameters             7
_refine_ls_number_restraints             0
_refine_ls_number_constraints            3
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(I)+0.0010394176I²)'
_refine_ls_hydrogen_treatment            .
_refine_ls_shift/su_max                  0.0000
_refine_ls_shift/su_mean                 0.0000
_refine_diff_density_max                 0.08
_refine_diff_density_min                 -0.13
_refine_ls_extinction_method             'SHELXL-2017/1 (Sheldrick, 2015)'
_refine_ls_extinction_coef               4.6(3)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'

loop_
 _atom_type_symbol
 _atom_type_scat_length_neutron
 _atom_type_scat_source
 Ba    5.070 International_Tables_Vol_C
 F     5.654 International_Tables_Vol_C
 Li   -1.900 International_Tables_Vol_C
 O     5.803 International_Tables_Vol_C

_atom_sites_solution_primary             iterative
_atom_sites_solution_secondary           .
_atom_sites_solution_hydrogens           .

_computing_data_collection               'NOMAD (Institut Laue-Langevin, 2016)'
_computing_cell_refinement               'RAFD9 (Filhol, 1988)'
_computing_data_reduction
 'RACER (Lehmann & Larsen, 1974; Wilkinson et al., 1988)'
_computing_structure_solution          'SUPERFLIP (Palatinus & Chapuis, 2007)'
_computing_structure_refinement        'Jana2006 (Petříček et al., 2014)'
_computing_molecular_graphics          'VESTA (Momma & Izumi, 2011)'
_computing_publication_material        'Jana2006 (Petříček et al., 2014)'

#=======================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
 _atom_site_constraints
  Ba1 Ba 0 0 0 Uani 0.02649(10) 1 1 d STP . . .
  Li1 Li 0.5 0.5 0.5 Uani 0.0368(2) 1 1 d STP . . .
  F1 F 0.5 0.5 0 Uani 0.03918(12) 3 0.9333 d STP . 1 .
  O1 O 0.5 0.5 0 Uani 0.03918(12) 3 0.0333 d STP . 2 'U=U(F1)'


loop_
 _jana_atom_site_ADP_C_label
 _jana_atom_site_ADP_C_type_symbol
 _jana_atom_site_ADP_C_111
 _jana_atom_site_ADP_C_112
 _jana_atom_site_ADP_C_113
 _jana_atom_site_ADP_C_122
 _jana_atom_site_ADP_C_123
 _jana_atom_site_ADP_C_133
 _jana_atom_site_ADP_C_222
 _jana_atom_site_ADP_C_223
 _jana_atom_site_ADP_C_233
 _jana_atom_site_ADP_C_333
 F1 F 0 0 0 0 0 0 0 0 0 0
 O1 O 0 0 0 0 0 0 0 0 0 0

loop_
 _jana_atom_site_ADP_D_label
 _jana_atom_site_ADP_D_type_symbol
 _jana_atom_site_ADP_D_1111
 _jana_atom_site_ADP_D_1112
 _jana_atom_site_ADP_D_1113
 _jana_atom_site_ADP_D_1122
 _jana_atom_site_ADP_D_1123
 _jana_atom_site_ADP_D_1133
 _jana_atom_site_ADP_D_1222
 _jana_atom_site_ADP_D_1223
 _jana_atom_site_ADP_D_1233
 _jana_atom_site_ADP_D_1333
 _jana_atom_site_ADP_D_2222
 _jana_atom_site_ADP_D_2223
 _jana_atom_site_ADP_D_2233
 _jana_atom_site_ADP_D_2333
 _jana_atom_site_ADP_D_3333
 F1 F 0 0 0 -0.0043(11) 0 0 0 0 0 0 0 0 0 0 0
 O1 O 0 0 0 -0.0043(11) 0 0 0 0 0 0 0 0 0 0 0

#=======================================================================

# MOLECULAR GEOMETRY

loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Ba1 F1 . 1_445 2.8824(4) ?
  Ba1 F1 . 1_455 2.8824(4) ?
  Ba1 F1 . 1_545 2.8824(4) ?
  Ba1 F1 . . 2.8824(4) ?
  Ba1 F1 . 5_544 2.8824(4) ?
  Ba1 F1 . 5_545 2.8824(4) ?
  Ba1 F1 . 5_554 2.8824(4) ?
  Ba1 F1 . 5_555 2.8824(4) ?
  Ba1 F1 . 9_454 2.8824(4) ?
  Ba1 F1 . 9_455 2.8824(4) ?
  Ba1 F1 . 9_554 2.8824(4) ?
  Ba1 F1 . 9_555 2.8824(4) ?
  Ba1 O1 . 1_445 2.8824(4) ?
  Ba1 O1 . 1_455 2.8824(4) ?
  Ba1 O1 . 1_545 2.8824(4) ?
  Ba1 O1 . . 2.8824(4) ?
  Ba1 O1 . 5_544 2.8824(4) ?
  Ba1 O1 . 5_545 2.8824(4) ?
  Ba1 O1 . 5_554 2.8824(4) ?
  Ba1 O1 . 5_555 2.8824(4) ?
  Ba1 O1 . 9_454 2.8824(4) ?
  Ba1 O1 . 9_455 2.8824(4) ?
  Ba1 O1 . 9_554 2.8824(4) ?
  Ba1 O1 . 9_555 2.8824(4) ?
  Li1 F1 . . 2.0382(4) ?
  Li1 F1 . 1_556 2.0382(4) ?
  Li1 F1 . 5_555 2.0382(4) ?
  Li1 F1 . 5_655 2.0382(4) ?
  Li1 F1 . 9_555 2.0382(4) ?
  Li1 F1 . 9_565 2.0382(4) ?
  Li1 O1 . . 2.0382(4) ?
  Li1 O1 . 1_556 2.0382(4) ?
  Li1 O1 . 5_555 2.0382(4) ?
  Li1 O1 . 5_655 2.0382(4) ?
  Li1 O1 . 9_555 2.0382(4) ?
  Li1 O1 . 9_565 2.0382(4) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  F1 Ba1 F1 1_445 . 1_455 90.000(8) ?
  F1 Ba1 F1 1_445 . 1_545 90.000(8) ?
  F1 Ba1 F1 1_445 . . 180 ?
  F1 Ba1 F1 1_445 . 5_544 60.000(4) ?
  F1 Ba1 F1 1_445 . 5_545 60.000(4) ?
  F1 Ba1 F1 1_445 . 5_554 120.000(4) ?
  F1 Ba1 F1 1_445 . 5_555 120.000(4) ?
  F1 Ba1 F1 1_445 . 9_454 60.000(4) ?
  F1 Ba1 F1 1_445 . 9_455 60.000(4) ?
  F1 Ba1 F1 1_445 . 9_554 120.000(4) ?
  F1 Ba1 F1 1_445 . 9_555 120.000(4) ?
  F1 Ba1 F1 1_455 . 1_545 180 ?
  F1 Ba1 F1 1_455 . . 90.000(8) ?
  F1 Ba1 F1 1_455 . 5_544 120.000(4) ?
  F1 Ba1 F1 1_455 . 5_545 120.000(4) ?
  F1 Ba1 F1 1_455 . 5_554 60.000(4) ?
  F1 Ba1 F1 1_455 . 5_555 60.000(4) ?
  F1 Ba1 F1 1_455 . 9_454 60.000(4) ?
  F1 Ba1 F1 1_455 . 9_455 60.000(4) ?
  F1 Ba1 F1 1_455 . 9_554 120.000(4) ?
  F1 Ba1 F1 1_455 . 9_555 120.000(4) ?
  F1 Ba1 F1 1_545 . . 90.000(8) ?
  F1 Ba1 F1 1_545 . 5_544 60.000(4) ?
  F1 Ba1 F1 1_545 . 5_545 60.000(4) ?
  F1 Ba1 F1 1_545 . 5_554 120.000(4) ?
  F1 Ba1 F1 1_545 . 5_555 120.000(4) ?
  F1 Ba1 F1 1_545 . 9_454 120.000(4) ?
  F1 Ba1 F1 1_545 . 9_455 120.000(4) ?
  F1 Ba1 F1 1_545 . 9_554 60.000(4) ?
  F1 Ba1 F1 1_545 . 9_555 60.000(4) ?
  F1 Ba1 F1 . . 5_544 120.000(4) ?
  F1 Ba1 F1 . . 5_545 120.000(4) ?
  F1 Ba1 F1 . . 5_554 60.000(4) ?
  F1 Ba1 F1 . . 5_555 60.000(4) ?
  F1 Ba1 F1 . . 9_454 120.000(4) ?
  F1 Ba1 F1 . . 9_455 120.000(4) ?
  F1 Ba1 F1 . . 9_554 60.000(4) ?
  F1 Ba1 F1 . . 9_555 60.000(4) ?
  F1 Ba1 F1 5_544 . 5_545 90.000(8) ?
  F1 Ba1 F1 5_544 . 5_554 90.000(8) ?
  F1 Ba1 F1 5_544 . 5_555 180 ?
  F1 Ba1 F1 5_544 . 9_454 60.000(4) ?
  F1 Ba1 F1 5_544 . 9_455 120.000(4) ?
  F1 Ba1 F1 5_544 . 9_554 60.000(4) ?
  F1 Ba1 F1 5_544 . 9_555 120.000(4) ?
  F1 Ba1 F1 5_545 . 5_554 180 ?
  F1 Ba1 F1 5_545 . 5_555 90.000(8) ?
  F1 Ba1 F1 5_545 . 9_454 120.000(4) ?
  F1 Ba1 F1 5_545 . 9_455 60.000(4) ?
  F1 Ba1 F1 5_545 . 9_554 120.000(4) ?
  F1 Ba1 F1 5_545 . 9_555 60.000(4) ?
  F1 Ba1 F1 5_554 . 5_555 90.000(8) ?
  F1 Ba1 F1 5_554 . 9_454 60.000(4) ?
  F1 Ba1 F1 5_554 . 9_455 120.000(4) ?
  F1 Ba1 F1 5_554 . 9_554 60.000(4) ?
  F1 Ba1 F1 5_554 . 9_555 120.000(4) ?
  F1 Ba1 F1 5_555 . 9_454 120.000(4) ?
  F1 Ba1 F1 5_555 . 9_455 60.000(4) ?
  F1 Ba1 F1 5_555 . 9_554 120.000(4) ?
  F1 Ba1 F1 5_555 . 9_555 60.000(4) ?
  F1 Ba1 F1 9_454 . 9_455 90.000(8) ?
  F1 Ba1 F1 9_454 . 9_554 90.000(8) ?
  F1 Ba1 F1 9_454 . 9_555 180 ?
  F1 Ba1 F1 9_455 . 9_554 180 ?
  F1 Ba1 F1 9_455 . 9_555 90.000(8) ?
  F1 Ba1 F1 9_554 . 9_555 90.000(8) ?
  O1 Ba1 O1 1_445 . 1_455 90.000(8) ?
  O1 Ba1 O1 1_445 . 1_545 90.000(8) ?
  O1 Ba1 O1 1_445 . . 180 ?
  O1 Ba1 O1 1_445 . 5_544 60.000(4) ?
  O1 Ba1 O1 1_445 . 5_545 60.000(4) ?
  O1 Ba1 O1 1_445 . 5_554 120.000(4) ?
  O1 Ba1 O1 1_445 . 5_555 120.000(4) ?
  O1 Ba1 O1 1_445 . 9_454 60.000(4) ?
  O1 Ba1 O1 1_445 . 9_455 60.000(4) ?
  O1 Ba1 O1 1_445 . 9_554 120.000(4) ?
  O1 Ba1 O1 1_445 . 9_555 120.000(4) ?
  O1 Ba1 O1 1_455 . 1_545 180 ?
  O1 Ba1 O1 1_455 . . 90.000(8) ?
  O1 Ba1 O1 1_455 . 5_544 120.000(4) ?
  O1 Ba1 O1 1_455 . 5_545 120.000(4) ?
  O1 Ba1 O1 1_455 . 5_554 60.000(4) ?
  O1 Ba1 O1 1_455 . 5_555 60.000(4) ?
  O1 Ba1 O1 1_455 . 9_454 60.000(4) ?
  O1 Ba1 O1 1_455 . 9_455 60.000(4) ?
  O1 Ba1 O1 1_455 . 9_554 120.000(4) ?
  O1 Ba1 O1 1_455 . 9_555 120.000(4) ?
  O1 Ba1 O1 1_545 . . 90.000(8) ?
  O1 Ba1 O1 1_545 . 5_544 60.000(4) ?
  O1 Ba1 O1 1_545 . 5_545 60.000(4) ?
  O1 Ba1 O1 1_545 . 5_554 120.000(4) ?
  O1 Ba1 O1 1_545 . 5_555 120.000(4) ?
  O1 Ba1 O1 1_545 . 9_454 120.000(4) ?
  O1 Ba1 O1 1_545 . 9_455 120.000(4) ?
  O1 Ba1 O1 1_545 . 9_554 60.000(4) ?
  O1 Ba1 O1 1_545 . 9_555 60.000(4) ?
  O1 Ba1 O1 . . 5_544 120.000(4) ?
  O1 Ba1 O1 . . 5_545 120.000(4) ?
  O1 Ba1 O1 . . 5_554 60.000(4) ?
  O1 Ba1 O1 . . 5_555 60.000(4) ?
  O1 Ba1 O1 . . 9_454 120.000(4) ?
  O1 Ba1 O1 . . 9_455 120.000(4) ?
  O1 Ba1 O1 . . 9_554 60.000(4) ?
  O1 Ba1 O1 . . 9_555 60.000(4) ?
  O1 Ba1 O1 5_544 . 5_545 90.000(8) ?
  O1 Ba1 O1 5_544 . 5_554 90.000(8) ?
  O1 Ba1 O1 5_544 . 5_555 180 ?
  O1 Ba1 O1 5_544 . 9_454 60.000(4) ?
  O1 Ba1 O1 5_544 . 9_455 120.000(4) ?
  O1 Ba1 O1 5_544 . 9_554 60.000(4) ?
  O1 Ba1 O1 5_544 . 9_555 120.000(4) ?
  O1 Ba1 O1 5_545 . 5_554 180 ?
  O1 Ba1 O1 5_545 . 5_555 90.000(8) ?
  O1 Ba1 O1 5_545 . 9_454 120.000(4) ?
  O1 Ba1 O1 5_545 . 9_455 60.000(4) ?
  O1 Ba1 O1 5_545 . 9_554 120.000(4) ?
  O1 Ba1 O1 5_545 . 9_555 60.000(4) ?
  O1 Ba1 O1 5_554 . 5_555 90.000(8) ?
  O1 Ba1 O1 5_554 . 9_454 60.000(4) ?
  O1 Ba1 O1 5_554 . 9_455 120.000(4) ?
  O1 Ba1 O1 5_554 . 9_554 60.000(4) ?
  O1 Ba1 O1 5_554 . 9_555 120.000(4) ?
  O1 Ba1 O1 5_555 . 9_454 120.000(4) ?
  O1 Ba1 O1 5_555 . 9_455 60.000(4) ?
  O1 Ba1 O1 5_555 . 9_554 120.000(4) ?
  O1 Ba1 O1 5_555 . 9_555 60.000(4) ?
  O1 Ba1 O1 9_454 . 9_455 90.000(8) ?
  O1 Ba1 O1 9_454 . 9_554 90.000(8) ?
  O1 Ba1 O1 9_454 . 9_555 180 ?
  O1 Ba1 O1 9_455 . 9_554 180 ?
  O1 Ba1 O1 9_455 . 9_555 90.000(8) ?
  O1 Ba1 O1 9_554 . 9_555 90.000(8) ?
  F1 Li1 F1 . . 1_556 180 ?
  F1 Li1 F1 . . 5_555 90 ?
  F1 Li1 F1 . . 5_655 90 ?
  F1 Li1 F1 . . 9_555 90 ?
  F1 Li1 F1 . . 9_565 90 ?
  F1 Li1 F1 1_556 . 5_555 90 ?
  F1 Li1 F1 1_556 . 5_655 90 ?
  F1 Li1 F1 1_556 . 9_555 90 ?
  F1 Li1 F1 1_556 . 9_565 90 ?
  F1 Li1 F1 5_555 . 5_655 180 ?
  F1 Li1 F1 5_555 . 9_555 90 ?
  F1 Li1 F1 5_555 . 9_565 90 ?
  F1 Li1 F1 5_655 . 9_555 90 ?
  F1 Li1 F1 5_655 . 9_565 90 ?
  F1 Li1 F1 9_555 . 9_565 180 ?
  O1 Li1 O1 . . 1_556 180 ?
  O1 Li1 O1 . . 5_555 90 ?
  O1 Li1 O1 . . 5_655 90 ?
  O1 Li1 O1 . . 9_555 90 ?
  O1 Li1 O1 . . 9_565 90 ?
  O1 Li1 O1 1_556 . 5_555 90 ?
  O1 Li1 O1 1_556 . 5_655 90 ?
  O1 Li1 O1 1_556 . 9_555 90 ?
  O1 Li1 O1 1_556 . 9_565 90 ?
  O1 Li1 O1 5_555 . 5_655 180 ?
  O1 Li1 O1 5_555 . 9_555 90 ?
  O1 Li1 O1 5_555 . 9_565 90 ?
  O1 Li1 O1 5_655 . 9_555 90 ?
  O1 Li1 O1 5_655 . 9_565 90 ?
  O1 Li1 O1 9_555 . 9_565 180 ?

#=======================================================================

# STRUCTURE-FACTOR LIST


#=======================================================================

# REFINEMENT INSTRUCTION FILE


#=======================================================================
data_BaLiF3-XRD
#=======================================================================

_database_code_CSD                       434518

# CHEMICAL DATA

_chemical_name_systematic                'barium lithium fluoride oxide'
_chemical_name_structure_type            Perovskite-CaTiO₃
_chemical_formula_iupac                  'Ba Li F2.80 O0.10'
_chemical_formula_sum                    'Ba F2.80 Li O0.10'
_chemical_formula_weight                 199.1
_chemical_compound_source                synthetic

#=======================================================================

# CRYSTAL DATA

_symmetry_cell_setting                   cubic
_symmetry_space_group_name_H-M           'P m -3 m'
_symmetry_space_group_name_Hall          '-P 4 2 3'
_symmetry_Int_Tables_number              221

loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -x,-y,z
 3   -x,y,-z
 4   x,-y,-z
 5   z,x,y
 6   z,-x,-y
 7   -z,-x,y
 8   -z,x,-y
 9   y,z,x
 10  -y,z,-x
 11  y,-z,-x
 12  -y,-z,x
 13  y,x,-z
 14  -y,-x,-z
 15  y,-x,z
 16  -y,x,z
 17  x,z,-y
 18  -x,z,y
 19  -x,-z,-y
 20  x,-z,y
 21  z,y,-x
 22  z,-y,x
 23  -z,y,x
 24  -z,-y,-x
 25  -x,-y,-z
 26  x,y,-z
 27  x,-y,z
 28  -x,y,z
 29  -z,-x,-y
 30  -z,x,y
 31  z,x,-y
 32  z,-x,y
 33  -y,-z,-x
 34  y,-z,x
 35  -y,z,x
 36  y,z,-x
 37  -y,-x,z
 38  y,x,z
 39  -y,x,-z
 40  y,-x,-z
 41  -x,-z,y
 42  x,-z,-y
 43  x,z,y
 44  -x,z,-y
 45  -z,-y,x
 46  -z,y,-x
 47  z,-y,-x
 48  z,y,x

_cell_length_a                           3.9970(8)
_cell_length_b                           3.9970(8)
_cell_length_c                           3.9970(8)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        90
_cell_volume                             63.86(4)
_cell_formula_units_Z                    1

_cell_measurement_temperature            279(2)
_cell_measurement_reflns_used            3487
_cell_measurement_theta_min              5.10
_cell_measurement_theta_max              30.19

_exptl_crystal_density_diffrn            5.1768
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            'not measured'
_exptl_crystal_F_000                     85

_exptl_absorpt_coefficient_mu            15.347
_exptl_crystal_description               shard
_exptl_crystal_size_min                  0.100
_exptl_crystal_size_mid                  0.212
_exptl_crystal_size_max                  0.329
_exptl_crystal_colour                    colourless
_exptl_absorpt_correction_type           numerical
_exptl_absorpt_process_details           'SADABS 2014/5 (Bruker, 2001)'
_exptl_absorpt_correction_T_max          0.0885
_exptl_absorpt_correction_T_min          0.0195

loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
   -2.00    9.00    0.00    0.0230
    1.00   -7.00    6.00    0.0660
   -9.00   -1.00    1.00    0.1340
    8.00    2.00   -3.00    0.1450
    0.00    2.00    9.00    0.0960
    0.00   -3.00   -1.00    0.0810
    1.00    9.00    5.00    0.0570
    3.00    0.00    1.00    0.1750
    7.00   -3.00   -8.00    0.1590
    0.00    9.00   -1.00    0.0140
   -1.00    0.00   -6.00    0.0850
    1.00   -9.00    1.00    0.0500
   -1.00   -6.00    1.00    0.0640
    1.00   -4.00    0.00    0.0600
   -6.00   -9.00   -4.00    0.1000
    0.00   -1.00    0.00    0.0600

#=======================================================================

# EXPERIMENTAL DATA

_exptl_special_details
;
 The following wavelength and cell were deduced by SADABS from the
 direction cosines etc. They are given here for emergency use only:
 CELL 0.71073    3.996    3.997    3.998   89.999   89.987   90.014
;

_diffrn_ambient_temperature              279(2)
_diffrn_ambient_environment              N~2~
_diffrn_source                           'micro-focus sealed tube'
_diffrn_source_type                      'Bruker I\mS 3.0'
_diffrn_radiation_probe                  x-ray
_diffrn_radiation_type                   'Mo K\a'
_diffrn_radiation_source                 'X-ray tube'
_diffrn_radiation_wavelength             0.71075
_diffrn_radiation_monochromator          graphite
_diffrn_measurement_device               'κ-geometry diffractometer'
_diffrn_measurement_device_type          'Bruker D8 VENTURE'
_diffrn_measurement_method               'φ and ω scans'
_diffrn_measurement_specimen_support     'polymer loop'
_diffrn_detector                         'pixel array detector'
_diffrn_detector_type                    'Bruker PHOTON II CPAD'
_diffrn_detector_area_resol_mean         7.376

_diffrn_reflns_number                    2602
_diffrn_reflns_theta_min                 5.1
_diffrn_reflns_theta_max                 30.2
_diffrn_reflns_theta_full                30.2
_diffrn_measured_fraction_theta_max      1
_diffrn_measured_fraction_theta_full     1
_diffrn_reflns_av_R_equivalents          0.0573
_diffrn_reflns_av_unetI/netI             0.0115
_diffrn_reflns_limit_h_min               -5
_diffrn_reflns_limit_h_max               5
_diffrn_reflns_limit_k_min               -5
_diffrn_reflns_limit_k_max               5
_diffrn_reflns_limit_l_min               -5
_diffrn_reflns_limit_l_max               5

_diffrn_standards_number                 0
_diffrn_standards_interval_count         .
_diffrn_standards_interval_time          .
_diffrn_standards_decay_%                ?

#=======================================================================

# REFINEMENT DATA

_refine_special_details
;
Substitutionally disordered fluoride and oxide ions were constrained
 to have the same ADP.
;

_reflns_number_total                     34
_reflns_number_gt                        34
_reflns_threshold_expression             I>2σ(I)

_refine_ls_structure_factor_coef         Fsqd
_refine_ls_matrix_type                   full
_refine_ls_R_factor_gt                   0.0097
_refine_ls_wR_factor_gt                  0.0225
_refine_ls_R_factor_all                  0.0097
_refine_ls_wR_factor_ref                 0.0225
_refine_ls_goodness_of_fit_ref           1.09
_refine_ls_goodness_of_fit_gt            1.09
_refine_ls_number_reflns                 34
_refine_ls_number_parameters             6
_refine_ls_number_restraints             0
_refine_ls_number_constraints            2
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(I)+0.0004177936I²)'
_refine_ls_hydrogen_treatment            ?
_refine_ls_shift/su_max                  0.0000
_refine_ls_shift/su_mean                 0.0000
_refine_diff_density_max                 0.73
_refine_diff_density_min                 -0.50
_refine_ls_extinction_method
 'B-C type 1 Lorentzian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef               5300(500)


loop_
 _atom_type_symbol
 _atom_type_oxidation_number
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 Ba   2  -0.3244  2.2819
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 F   -1   0.0171  0.0103
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Li   1  -0.0003  0.0001
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 O   -2   0.0106  0.0060
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_atom_sites_solution_primary             iterative
_atom_sites_solution_secondary           .
_atom_sites_solution_hydrogens           .

_computing_data_collection               'Bruker APEX2 (Bruker, 2012)'
_computing_cell_refinement               'Bruker SAINT (Bruker, 2012)'
_computing_data_reduction                'Bruker SAINT (Bruker, 2012)'
_computing_structure_solution            'SUPERFLIP (Palatinus & Chapuis, 2007)'
_computing_structure_refinement        'Jana2006 (Petříček et al., 2014)'
_computing_molecular_graphics            'VESTA (Momma & Izumi, 2011)'
_computing_publication_material        'Jana2006 (Petříček et al., 2014)'

#=======================================================================

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
 _atom_site_constraints
  Ba1 Ba 0 0 0 Uani 0.0076(3) 1 1 d STP . . .
  F1 F 0.5 0 0.5 Uani 0.0124(9) 3 0.9333 d STP . 1 .
  O1 O 0.5 0 0.5 Uani 0.0124(9) 3 0.0333 d STP . 2 'U=U(F1)'
  Li1 Li 0.5 0.5 0.5 Uani 0.012(2) 1 1 d STP . . .


#=======================================================================

# MOLECULAR GEOMETRY

loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Ba1 O1 . 1_454 2.8263(8) ?
  Ba1 O1 . 1_455 2.8263(8) ?
  Ba1 O1 . 1_554 2.8263(8) ?
  Ba1 O1 . . 2.8263(8) ?
  Ba1 O1 . 5_445 2.8263(8) ?
  Ba1 O1 . 5_455 2.8263(8) ?
  Ba1 O1 . 5_545 2.8263(8) ?
  Ba1 O1 . 5_555 2.8263(8) ?
  Ba1 O1 . 9_544 2.8263(8) ?
  Ba1 O1 . 9_545 2.8263(8) ?
  Ba1 O1 . 9_554 2.8263(8) ?
  Ba1 O1 . 9_555 2.8263(8) ?
  Li1 F1 . . 1.9985(8) ?
  Li1 F1 . 1_565 1.9985(8) ?
  Li1 F1 . 5_555 1.9985(8) ?
  Li1 F1 . 5_556 1.9985(8) ?
  Li1 F1 . 9_555 1.9985(8) ?
  Li1 F1 . 9_655 1.9985(8) ?
  Li1 O1 . . 1.9985(8) ?
  Li1 O1 . 1_565 1.9985(8) ?
  Li1 O1 . 5_555 1.9985(8) ?
  Li1 O1 . 5_556 1.9985(8) ?
  Li1 O1 . 9_555 1.9985(8) ?
  Li1 O1 . 9_655 1.9985(8) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  O1 Ba1 O1 1_454 . 1_455 90.000(16) ?
  O1 Ba1 O1 1_454 . 1_554 90.000(16) ?
  O1 Ba1 O1 1_454 . . 180 ?
  O1 Ba1 O1 1_454 . 5_445 60.000(8) ?
  O1 Ba1 O1 1_454 . 5_455 60.000(8) ?
  O1 Ba1 O1 1_454 . 5_545 120.000(8) ?
  O1 Ba1 O1 1_454 . 5_555 120.000(8) ?
  O1 Ba1 O1 1_454 . 9_544 60.000(8) ?
  O1 Ba1 O1 1_454 . 9_545 120.000(8) ?
  O1 Ba1 O1 1_454 . 9_554 60.000(8) ?
  O1 Ba1 O1 1_454 . 9_555 120.000(8) ?
  O1 Ba1 O1 1_455 . 1_554 180 ?
  O1 Ba1 O1 1_455 . . 90.000(16) ?
  O1 Ba1 O1 1_455 . 5_445 60.000(8) ?
  O1 Ba1 O1 1_455 . 5_455 60.000(8) ?
  O1 Ba1 O1 1_455 . 5_545 120.000(8) ?
  O1 Ba1 O1 1_455 . 5_555 120.000(8) ?
  O1 Ba1 O1 1_455 . 9_544 120.000(8) ?
  O1 Ba1 O1 1_455 . 9_545 60.000(8) ?
  O1 Ba1 O1 1_455 . 9_554 120.000(8) ?
  O1 Ba1 O1 1_455 . 9_555 60.000(8) ?
  O1 Ba1 O1 1_554 . . 90.000(16) ?
  O1 Ba1 O1 1_554 . 5_445 120.000(8) ?
  O1 Ba1 O1 1_554 . 5_455 120.000(8) ?
  O1 Ba1 O1 1_554 . 5_545 60.000(8) ?
  O1 Ba1 O1 1_554 . 5_555 60.000(8) ?
  O1 Ba1 O1 1_554 . 9_544 60.000(8) ?
  O1 Ba1 O1 1_554 . 9_545 120.000(8) ?
  O1 Ba1 O1 1_554 . 9_554 60.000(8) ?
  O1 Ba1 O1 1_554 . 9_555 120.000(8) ?
  O1 Ba1 O1 . . 5_445 120.000(8) ?
  O1 Ba1 O1 . . 5_455 120.000(8) ?
  O1 Ba1 O1 . . 5_545 60.000(8) ?
  O1 Ba1 O1 . . 5_555 60.000(8) ?
  O1 Ba1 O1 . . 9_544 120.000(8) ?
  O1 Ba1 O1 . . 9_545 60.000(8) ?
  O1 Ba1 O1 . . 9_554 120.000(8) ?
  O1 Ba1 O1 . . 9_555 60.000(8) ?
  O1 Ba1 O1 5_445 . 5_455 90.000(16) ?
  O1 Ba1 O1 5_445 . 5_545 90.000(16) ?
  O1 Ba1 O1 5_445 . 5_555 180 ?
  O1 Ba1 O1 5_445 . 9_544 60.000(8) ?
  O1 Ba1 O1 5_445 . 9_545 60.000(8) ?
  O1 Ba1 O1 5_445 . 9_554 120.000(8) ?
  O1 Ba1 O1 5_445 . 9_555 120.000(8) ?
  O1 Ba1 O1 5_455 . 5_545 180 ?
  O1 Ba1 O1 5_455 . 5_555 90.000(16) ?
  O1 Ba1 O1 5_455 . 9_544 120.000(8) ?
  O1 Ba1 O1 5_455 . 9_545 120.000(8) ?
  O1 Ba1 O1 5_455 . 9_554 60.000(8) ?
  O1 Ba1 O1 5_455 . 9_555 60.000(8) ?
  O1 Ba1 O1 5_545 . 5_555 90.000(16) ?
  O1 Ba1 O1 5_545 . 9_544 60.000(8) ?
  O1 Ba1 O1 5_545 . 9_545 60.000(8) ?
  O1 Ba1 O1 5_545 . 9_554 120.000(8) ?
  O1 Ba1 O1 5_545 . 9_555 120.000(8) ?
  O1 Ba1 O1 5_555 . 9_544 120.000(8) ?
  O1 Ba1 O1 5_555 . 9_545 120.000(8) ?
  O1 Ba1 O1 5_555 . 9_554 60.000(8) ?
  O1 Ba1 O1 5_555 . 9_555 60.000(8) ?
  O1 Ba1 O1 9_544 . 9_545 90.000(16) ?
  O1 Ba1 O1 9_544 . 9_554 90.000(16) ?
  O1 Ba1 O1 9_544 . 9_555 180 ?
  O1 Ba1 O1 9_545 . 9_554 180 ?
  O1 Ba1 O1 9_545 . 9_555 90.000(16) ?
  O1 Ba1 O1 9_554 . 9_555 90.000(16) ?
  F1 Li1 F1 . . 1_565 180 ?
  F1 Li1 F1 . . 5_555 90 ?
  F1 Li1 F1 . . 5_556 90 ?
  F1 Li1 F1 . . 9_555 90 ?
  F1 Li1 F1 . . 9_655 90 ?
  F1 Li1 F1 1_565 . 5_555 90 ?
  F1 Li1 F1 1_565 . 5_556 90 ?
  F1 Li1 F1 1_565 . 9_555 90 ?
  F1 Li1 F1 1_565 . 9_655 90 ?
  F1 Li1 F1 5_555 . 5_556 180 ?
  F1 Li1 F1 5_555 . 9_555 90 ?
  F1 Li1 F1 5_555 . 9_655 90 ?
  F1 Li1 F1 5_556 . 9_555 90 ?
  F1 Li1 F1 5_556 . 9_655 90 ?
  F1 Li1 F1 9_555 . 9_655 180 ?
  O1 Li1 O1 . . 1_565 180 ?
  O1 Li1 O1 . . 5_555 90 ?
  O1 Li1 O1 . . 5_556 90 ?
  O1 Li1 O1 . . 9_555 90 ?
  O1 Li1 O1 . . 9_655 90 ?
  O1 Li1 O1 1_565 . 5_555 90 ?
  O1 Li1 O1 1_565 . 5_556 90 ?
  O1 Li1 O1 1_565 . 9_555 90 ?
  O1 Li1 O1 1_565 . 9_655 90 ?
  O1 Li1 O1 5_555 . 5_556 180 ?
  O1 Li1 O1 5_555 . 9_555 90 ?
  O1 Li1 O1 5_555 . 9_655 90 ?
  O1 Li1 O1 5_556 . 9_555 90 ?
  O1 Li1 O1 5_556 . 9_655 90 ?
  O1 Li1 O1 9_555 . 9_655 180 ?

#=======================================================================

# STRUCTURE-FACTOR LIST


#=======================================================================

# REFINEMENT INSTRUCTION FILE



